Heat Treatment Processes
It is a process of heating cycles where the
metal is subjected to controlled temperature
changes in solid state. Heating process can
change the size and shape of grain structure
and can also change the constituents and
hence the properties of steel.
Fe-C equilibrium diagram showing temperature ranges for various heat
Types of Heat Treatment
3. Quenching or Hardening
5. Surface Hardening
6. Case Hardening
Hardening Processes for Gears
There are mainly following 3 processes
which are used for hardening the gears
(1) Through Hardening
(2) Case Hardening:
(3) Surface Hardening:
(a) Induction Hardening,
(b) Flame Hardening.
This includes heating of the whole material to form austenite and
then cooling it the right medium to produce martensitic phase in it.
The process consists of general hardening process like quenching and
post process like tempering.
Through hardening should not be confused with constant hardness.
Hardness of material is not constant but a gradient of hardness exists.
Through hardened steels are used for gears carrying small
specific loads and are usually unalloyed or lean alloy steel. They
have lowest hardenability.
Examples of commonly Through Hardened gear steels are AISI
1045, 4130, 4140, 4145, 4340, 8640.
Case Hardening produces a hard, wear resistance
case or surface layer on the top of a ductile, shock
resistance interior or core.
The idea behind the case hardening is to keep the
core of the gear tooth at a level around 30 to 40
HRC to avoid tooth breakage while hardening the
outer surface to increase the pitting resistance
Case hardening consists of three processes:
Carburizing is a heat treatment process in which iron or steel
is heated in the presence of another material which liberates
carbon as it decomposes, at temperature between 850 and
950°C, at which austenite, with its high solubility for carbon,
is the stable crystal structure. Hardening is accomplished when
the high-carbon surface layer is quenched to form Martensite so
that a high-carbon martensitic case with good wear and fatigue
resistance is superimposed on a tough, low-carbon steel core.
Gears are almost always oil quenched because
distortion must be held to the lowest possible level.
After case hardening, the hardness obtained lies in the
range HRC 58 to 62 but in heavily loaded gears a minimum
of HRC 60 is required.
Nitriding is a surface-hardening heat treatment that
introduces nitrogen into the surface of steel at a
temperature range of 500 to 550°C, while it is in the
Because nitriding does not involve heating into the
austenite phase field and a subsequent quench to form
martensite, nitriding can be accomplished with a minimum of
distortion and with excellent dimensional control.
Nitriding is done to to obtain high surface hardness,
increase wear resistance, improve fatigue life, improve
corrosion resistance (except for stainless steels), obtain a
surface that is resistant to the softening effect of heat at
temperatures up to the nitriding temperature.
Carbonitriding is one of most common type of case hardening
processes for gears
Carbonitriding is essentially a modified version of gas carburizing.
The modification consists of bringing in ammonia into the gas
carburizing atmosphere. This adds nitrogen to the carburized case.
The nitrogen gets diffused simultaneously into the steel along with
Generally a carbonitriding process is done at a lower temperature
and for a quicker span of time than that of gas carburizing.
It has been found that after Carbo-Nitriding of Gears there has
been considerable improvement in useful life for many of the
gears. Advantages for gears include temper resistance,
heightened lubricity during cold start, better strength of the
base metal in terms of tensile, yield and fatigue, an increase in
throughput, also elimination of problems like quench cracking.
This is a special hardening process in
which a particular surface of steel is
made hard without altering the hardness
of any other portion.
There are two types of surface
1. Induction Hardening
2. Flame Hardening
Induction hardening is a heat treating technique that can be used
to selectively harden portions of a gear, such as the flanks, roots
and tips of teeth, providing improved hardness, wear resistance,
and contact fatigue strength without affecting the metallurgy of the
core and other parts of the component that don’t require change.
Induction hardening does not require heating the whole gear.
With induction, heating can be localized to only those areas
in which metallurgical changes are required. For example,
the flanks, roots and tips of gear teeth can be selectively
A major goal of induction gear hardening is to provide a finegrain
martensitic layer on specific areas of the part.
External spur and helical gears, worm gears and internal
gears, bevel gears, racks and sprockets are among the parts
that are typically induction hardened.
The flame hardening of gear teeth is a sound investment since it
increases the life of the gear by about 5 times.
Flame hardening decreases both rolling friction and
deformation.Generally there are two methods of flame
hardening gear teeth - spin hardening or progressive
With spin hardening all the teeth are heated & then
quenched. With progressive hardening individual tooth flanks
are heated & quenched.
Flame hardening applies to most gear types - spur, helical,
bevel, spiral bevel, herringbone and racks.
A wide variety of materials may be flame hardened including
carbon and alloy steels, martensitic stainless steels and SG cast
irons. Generally steels with approximately 0.35-0.55 percent
carbon are suitable for flame hardening. Cast irons, higher
carbon and higher alloy steels are susceptible to cracking & extra
care should be taken to reduce this risk.
Flame Hardening In Gears
Flame hardening process in
By :- Kartik Thakkar